  Magnesium (Mg) and its alloys offer great potential for reducing vehicular
mass and energy consumption due to their inherently low densities.
Historically, widespread applicability has been limited by low strength
properties compared to other structural Al-, Ti- and Fe-based alloys. However,
recent studies have demonstrated high-specific-strength in a number of
nanocrystalline Mg-alloys. Even so, applications of these alloys would be
restricted to low-temperature automotive components due to microstructural
instability under high temperature creep loading. Hence, this work aims to gain
a better understanding of creep and associated deformation behavior of columnar
nanocrystalline Mg and Mg-yttrium (Y) (up to 3at.%Y(10wt.%Y)) with a grain size
of 5 nm and 10 nm. Using molecular dynamics (MD) simulations, nanocrystalline
magnesium with and without local concentrations of yttrium is subjected to
constant-stress loading ranging from 0 to 500 MPa at different initial
temperatures ranging from 473 to 723 K. In pure Mg, the analyses of the
diffusion coefficient and energy barrier reveal that at lower temperatures
(i.e., T < ~423K) the contribution of grain boundary diffusion to the overall
creep deformation is stronger that the contribution of lattice diffusion.
However, at higher temperatures (T > ~423K) lattice diffusion dominates the
overall creep behavior. Interestingly, for the first time, we have shown that
the(101-1),(101-2),(101-3) and (101-6) boundary sliding energy is reduced with
the addition of yttrium. This softening effect in the presence of yttrium
suggests that the experimentally observed high temperature beneficial effects
of yttrium addition is likely to be attributed to some combination of other
reported creep strengthening mechanisms or phenomena such as formation of
stable yttrium oxides at grain boundaries or increased forest dislocation-based
hardening.
